International Journal of Corrosion

Volume 2011, Article ID 761418, 12 pages

http://dx.doi.org/10.1155/2011/761418

## Inhibition Effect of 1-Butyl-4-Methylpyridinium Tetrafluoroborate on the Corrosion of Copper in Phosphate Solutions

Institute of Chemistry, UJK Kielce, Swietokrzyska Street15G, 25406 Kielce, Poland

Received 19 November 2010; Accepted 1 February 2011

Academic Editor: Flavio Deflorian

Copyright © 2011 M. Scendo and J. Uznanska. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

The influence of the concentration of 1-Butyl-4-methylpyridinium tetrafluoroborate (4MBPBF_{4}) as ionic liquid (IL) on the corrosion of copper in 0.5 M solutions of pH 2 and 4 was studied. The research involved electrochemical polarization method, and scanning electron microscopy (SEM) technique. The results obtained showed that the inhibition efficiency of corrosion of copper increases with an increase in the concentration of 4MBPBF_{4} but decreases with increasing temperature. The thermodynamic functions of corrosion analysis and adsorptive behavior of 4MBPBF_{4} were carried out. During the test, the adsorption of the inhibitor on the copper surface in the phosphate solutions was found to obey the Langmuir adsorption isotherm and had a physical mechanism.

#### 1. Introduction

Copper is used as a construction metal in the central heating installations, car industry, energetics, oil refineries, sugar factories, marine environment, to name only a few of its various applications. This extensive use of copper is due to its mechanical and electric properties as well as the behaviour of its passivation layer. Acidic solutions are widely used in various industries for the cleaning of copper. The behaviour of copper in acidic media is extensively investigated, and several ideas have been presented for the dissolution process [1, 2]. To avoid the base metal attack and to ensure the removal of corrosion products/scales alone, inhibitors are extensively used. The most well-known acid inhibitors are organic compounds containing nitrogen, phosphor, sulfur, and oxygen atoms. The surfactant inhibitors have many advantages such as high inhibition efficiency (IE), low price, low toxicity, and easy production [3–5]. The interactions between the inhibitor molecules and the metal surfaces should by all means be explained and understood in detail. In examining of these interactions, theoretical approaches applied can be very useful [6–10]. Many *N*-heterocyclic compounds have been used for the corrosion inhibition of metals, such as imidazoline [11], triazole [12–14], tetrazole [15], pyrrole [16], pyridine [17], pyrazole and bipyrazole [18, 19], pyrimidine [20], pyridazine [21], and some derivatives. Some heterocyclic compounds containing a mercapto group have been developed as copper corrosion inhibitors. These compounds include: 2-mercaptobenzothiazole [22], 2,4-dimercaptopyrimidine [23], 2-amino-5-mercaptothiadzole, 2-mercaptothiazoline [24], potassium ethyl xanthate [25–28] and indole and derivatives [29]. Among the numerous organic compounds tested and industrially applied as corrosion inhibitors, nontoxic onesare far more strategic now than in the recent past. These compounds include such amino acids [30–32] and derivatives as cysteine [33].

In the past two decades, the research in the field of *green* corrosion inhibitors has been addressed towards the goal of using cheap effective molecules at low or *zero* environmental impact. These compounds include purine and adenine, which have been tested for copper corrosion in chloride [34, 35], sulfate [36], and nitrate solutions [37].

Ionic liquids (ILs) are molten salts with melting points at/or below ambient temperature, which are composed of organic cations and various anions. Configuration of ILs consists of an amphiphilic group with a long chain, hydrophobic tail, and a hydrophilic polar head. Usually, ILs have nitrogen, sulphur, and phosphorus as the central atoms of cations, such as imidazolium, pyrrolidinium, quaternay ammonium, pyridinium, piperidinium, sulfonium and quaternary phosphonium. Currently, funtionalized IL is a very noticeable topic in the field of IL research. Introducing different functional groups into cations provides a great deal of ILs with new structures that can markedly change the physicochemical properties of ILs, and it also affords more choices for applications of ILs in electrochemical devices.

Imidazolium compounds are reported to show corrosion resistant behavior on mild steel [38], copper [39, 40], and aluminium [41]. It was found that the action of such inhibitors depends on the specific interaction between the functional groups and the metal surface, due to the presence of the –C = N– group and electronegative nitrogen in the molecule. Ionic liquids and different types of surfactans base inhibitors are well known to have a high activity in acid medium [42, 43] and therefore are used in an oil field to minimize carbon-dioxide-induced corrosion [44, 45]. Among many kinds of functionalized ionic liquids ether-functionalized ILs have been investigated intensively, and ether groups have been successfully introduced in to imidazolium cations [46–52].

However, no substantial information is available on pyridinium ionic liquids being used as corrosion inhibitors of copper.

The present work describes a study of the corrosion of copper in 0.5 M solutions of pH 2 and 4 without and with different concentrations of 1-Butyl-4-methylpyridinium tetrafluoroborate (4MBPBF_{4}), based on copper stationary disc electrode voltammetry measurements and scanning electron microscope. Moreover, the thermodynamic functions were appointed for the adsorption process and to gain more information about the mode of adsorption of the inhibitor on the surface of copper.

#### 2. Experimental Methods

##### 2.1. Solutions

1-Butyl-4-methylpyridinium tetrafluoroborate (4MBPBF_{4}) (>99.8%) was purchased from Fluka. The molecular structures of compound are shown in Figure 1. It is worth to notice that 4MBPBF_{4} is not flat molecule. The 4MBPBF_{4} is stable in air, water, and in majority organic solvents. However, this compound is well enough solvable in water. All the solutions were prepared using analytical grade reagent and triple distilled water (resistivity 13 MΩ cm). The 4MBPBF_{4} was dissolved at concentrations in the range of 1.0–50.0 mM in 0.5 M solutions of pH 2 and 4. During the measurements, the solution was not stirred or deaerated.

##### 2.2. Electrodes and Apparatus

The working electrode was a home-made stationary disk electrode (SDE) of Specpure copper (Johnson Matthey Chemicals Ltd.) with cm and cm^{2}. Prior to each experiment the working electrode was mechanically polished to mirror gloss by using 1000 and 2000-grade emery papers. Then the electrode was washed several times interchangeably with bidistilled water and ethanol. Finally, SDE was dried using a stream of air. Such pretreatment of the disk was repeated after each voltammetric measurement. Other details were published in [53–56]. All the surface-area-dependant values are normalized with respect to the geometric surface area of the working electrode.

Electrode potentials were measured and reported against the external saturated calomel electrode with NaCl solution (SCE(NaCl)) coupled with a fine Luggin capillary. To minimize the ohmic contribution, the capillary was kept close to the working electrode. A platinum (purity 99.99%) wire was used as an auxiliary electrode. Auxiliary electrode was individually isolated from the test solution by a glass frit.

All voltammetric experiments were performed using a Model EA9C electrochemical analyzer, controlled via Pentium computer using the software Eagraph V. 4.0.

##### 2.3. Scanning Electron Microscope

A scanning electron microscope (SEM) PHILIPS XL 30 was used to study the morphology of the copper surface in the absence and presence of the inhibitor. Samples were attached on top of an aluminum stopper by means of 3 M carbon conductive adhesive tape (SPI).

##### 2.4. Potentiodynamic Polarization Measurements

Electrochemical experiments were carried out in a classical three-electrode glass cell. The cell was open to air. The degreased SDE was quickly inserted into the solution and immediately cathodically polarized at −1100 mV (SCE(NaCl)) for 3 min to reduce any oxide on the copper surface. The polarization curves were obtained using the linear potential sweep (LSV) technique. The scan started from the cathodic (−1100 mV) to the anodic direction with the scan rate of 1 mV s^{−1}. Electrochemical experiments were repeated many times, and the average values of the current were used.

All experiments were carried out using an air thermostat with the forced air circulation.

#### 3. Experimental Results and Discussion

##### 3.1. Polarization Behaviour of Copper

The effect of 1-Butyl-4-methylpyridinium tetrafluoroborate (4MBPBF_{4}) on the corrosion reactions of copper was determined by polarization measurements at 20**°**C. Figure 2 shows example of polarization curves for the copper electrode in 0.5 M solutions of pH 4 without and with different concentrations of 4MBPBF_{4}. Similar curves were recorded for solution of pH 2. It is clear that the presence of different concentrations of the inhibitor decreases the current densities and reduces both of the cathodic and anodic current densities in comparison to those recorded in the additive-free solution. However, in case of more acid solutions (pH 2) were observed smaller changes in the cathodic and anodic current densities. The decrease in current densities could be attributed to the decrease in the phosphate ions attack on the copper surface due to the adsorption of the inhibitor molecules at the copper/solution interface.

###### 3.1.1. Corrosion Parameters

The corrosion kinetic parameters were calculated on the basis of cathodic and anodic potential versus current characteristics in the Tafel potential region (Figure 3). The corrosion parameters such as corrosion potential , corrosion current density , and cathodic and anodic Tafel slope are listed in Table 1. It is worth noticing that addition of the 4MBPBF_{4} causes more negative shift in corrosion potential values independently from pH solutions. Hence small changes in potentials can be a result of the competition of the cathodic and the anodic inhibiting reactions.

The corrosion current density (Table 1) decreased when the concentrations of 1-Butyl-4-methylpyridinium tetrafluoroborate were increased for both solutions of pH 2 and 4. This indicates the inhibiting effect of 4MBPBF_{4} on corrosion of copper. The decrease in cathodic and anodic or the increase in only in case of solutions of pH 4 Tafel slopes (Table 1) indicated that the 1-Butyl-4-methylpyridinium tetrafluoroborate molecules are adsorbed on both the anodic and cathodic sites resulting in an inhibition of both anodic dissolution of copper and cathodic reduction reactions. Moreover, these inhibitors cause small change in the cathodic and anodic Tafel slopes, indicating that 4MBPBF_{4} is first adsorbed onto copper surface and therefore impedes the reactionby merely blocking the reaction sites of copper surface without affecting the cathodic and anodic reaction mechanism [57].

###### 3.1.2. Polarization Resistance

The polarization resistance values are related to the corrosion current density , which can be calculated from the equation:
The values listed in Table 1 are used to estimate the corrosion inhibition effect of the inhibitor. The addition of 1-Butyl-4-methylpyridinium tetrafluoroborate to the phosphate solutions produced higher values than the blank solution indicating the formation of a protective layer on the electrode surface. Hence, the polarization resistance values increase with an increase in the concentration of 4MBPBF_{4} for both solutions of pH 2 and 4. It seems that protective layer created on surface of copper is the most tight in of less acid solution about the largest concentration of 1-Butyl-4-methylpyridinium tetrafluoroborate.

###### 3.1.3. Inhibition Efficiency

Inhibition efficiency (IE) can also be calculated from polarization tests by using the following equation [58, 59]: where and are the corrosion current densities in the absence and presence of inhibitor, respectively.

The inhibition efficiency depends on both the nature and the concentration of the investigated compounds. The calculated inhibition efficiencies are presented in Figure 4. In the presence of 1-Butyl-4-methylpyridinium tetrafluoroborate solution of pH 2 and 4, the inhibition efficiency increases with an increase in the concentration of inhibitor. This confirms the inhibiting character of 1-Butyl-4-methylpyridinium tetrafluoroborate. However, IE is higher in case of solution of pH 4 than 2. It is obvious that in the presence of 1-Butyl-4-methylpyridinium tetrafluoroborate solution of pH 2 the film on copper does not cover tightly the surface and hence does not protect it prior to corrosion of Cu in an adequate degree.

###### 3.1.4. Corrosion Rate

The corrosion current density was converted into the corrosion rate by using the expression [60]:
where is the molecular weight of copper, is the number of electrons transferred in the corrosion reaction, and is the density of Cu (g cm^{−3}).

The values of the copper corrosion rate in the absence and the presence of inhibitor for solution of both pH Values are presented in Table 2. The corrosion rate of copper is significantly reduced as a result of the reduction in the corrosion current densities. The protective layer on surface of metal causes that the corrosion rate to be more diminishes in case of less acid solution of phosphates.

##### 3.2. Scanning Electron Microscopy Studies

The surface morphology of copper samples immersed in 0.5 M (pH 2 and 4) for 24 hours in the absence and in the presence of 50.0 mM of 1-Butyl-4-methylpyridinium tetrafluoroborate was studied by scanning electron microscopy (SEM). The solutions were not degassed.

Figure 5 show the surface morphology of copper specimens (a) before and (b) after being immersed in corrosive solution (pH 2). The photograph (b) revels that the surface was strongly damaged in absence of the inhibitor. Figures 5(c) and 5(d) show SEM images of the surface copper specimens after immersion (for the same time interval) in corrosive solution containing additionally 50.0 mM of 1-Butyl-4-methylpyridinium tetrafluoroborate of pH 2 and 4, respectively. In the presence of the inhibitor the film precipitates on the surface of copper. The SEM photographs show that protective layer does not cover tightly the surface, and, hence does not protect the Cu surface to an adequate degree especially in case of solution of pH 2. Phosphate ions, oxygen and water penetrate the protective film through pores, flaws or other weak spots what results in the further corrosion of copper. In order to check the results of action by aggressive solution, the protective layer was removed from surface of copper. The layer was well adhered to the surface of the metal, and the removal of it was really difficult. Therefore ultrasonic water bath was used. The sample was shaken in diluted acetic acid and rinsed in propanol. Figure 5 presents samples after the removal of the inhibiting film for pH 4 (Figure 5(e)) and 2 (Figure 5(f)). However. However, received results indicated that more tight protective layer was forming in solution of pH 4 (Figure 5(e)). Moreover, in phosphate solution the 4MBPBF_{4} acts better as the inhibitor in less acidic environment.

##### 3.3. Mechanism of Corrosion Inhibition

Regarding the mechanism the oxygen reduction reaction on copper in acidic solutions a lot of work has been carried out [61–67]. The cathodic global reaction in an aerated aqueous phosphate solution could be described as follows: However, the first cathodic wave is attributed to reaction: In the more negative potential at the electrode, surface occurs thenext reaction: Furthermore, reaction (4a) is strongly influenced by potential [66].

The dissolution process of copper (anodic corrosion reaction) at low overpotentials runs according to the following steps [68–70]: where the is an adsorbed monovalent species of copper at the electrode surface.

The inhibition effect of 1-Butyl-4-methylpyridinium tetrafluoroborate on the copper surface could be explained as follows

The inhibitor of 4MBPBF_{4} can be protonated in acidic solutions:
Then the inhibitor molecules adsorb through electrostatic interactions between the negatively charged copper surface and positively charged [4MBPBHF_{4}]^{+}. However, the electrode carried the negative charge, therefore [4MBPBHF_{4}]^{+} ions should be first adsorbed directly on copper to probably form a protective layer at active sites: and blocks the further oxidation reaction of to Cu^{2+} (reaction (5b)). Moreover, the inhibitor molecules lead to the blocking of the transfer of oxygen from the bulk solution to the copper/solution interface that is going to reduce the cathodic reaction of oxygen (reaction (4a)). This indicates that the presence in phosphate solution of 4MBPBF_{4} affects both the cathodic and anodic reactions, therefore the, compound acts as a mixed-type inhibitor. The proposed mechanism of corrosion inhibition of copper by 4MBPBF_{4} in phosphate solutions (reactions (4a)-(5a)) requires the confirmation through making additional research.

However, exhausting information regarding mechanism of corrosion inhibition can be obtained on the basis of thermodynamic measurements.

##### 3.4. Effect of Temperature

The effect of temperature on the corrosion of copper in 0.5 M solution in the absence and presence of 10.0 mM of 1-Butyl-4-methylpyridinium tetrafluoroborate of pH 2 and 4 at temperature ranging from 303 to 343 K was investigated by potentiodynamic polarization measurements. The corrosion parameters and the inhibition efficiency are presented in Table 3. The corrosion potential and cathodic and anodic Tafel slope change similarly in case of low temperature of solutions (Table 1). Therefore, the growth of temperature of solutions does not influence the change of inhibition mechanism. Worth noticing is that the corrosion current density increases and inhibition efficiency decreases with increasing temperature, which indicates desorption of the inhibitor molecules from the surface of copper with rising temperature of solutions.

###### 3.4.1. Thermodynamic Activation Parameters

Thermodynamic activation parameters are important to study the inhibitive mechanism. The mechanism of the inhibitor action can be deduced by comparing the apparent activation energies, , in the presence and absence of the corrosion inhibitor. Activation parameters such as , the enthalpy of activation, , and the entropy of activation, , were calculated from an Arrhenius-type plot [71, 72]:
where is the Arrhenius constant, is the apparent activation energy, is the universal gas constant, and is the absolute temperature. An alternative formula of the Arrhenius equation is the transition state equation [73]:
where is the Avogadro’s constant, is the Planck’s constant, is the change of entropy for activation, and is the change of enthalpy for activation. Plots of versuss , and ln () versus give straight lines with slopes of and , respectively. The intercepts, which can then be calculated, will be for the Arrhenius and transition-state equations, respectively. Figures 6 and 7 represent the data plots in the absence and presence of 4MBPBF_{4} of pH 2 and 4. The calculated thermodynamic activation parameters are listed in Table 4. The values of and in the presence of 10.0 mM 4MBPBF_{4} are higher than those in black solutions, indicating that more energy barrier for the reaction in the presence of 4MBPBF_{4} is attained, especially in case of pH 4. This shows that the energy barrier of the corrosion reaction increased in the presence of the inhibitor without changing the mechanism of dissolution of copper [74]. The entropy of activation, , in the absence and presence of 4MBPBF_{4} is large and negative (especially with pH 4), implying that the rate-determining step for the activated complex is the association rather than the dissociation step, which means that a decrease in disordering takes place by going from reactants to the activated complex [75].

##### 3.5. Adsorption Isotherm

It has been assumed that inhibitor molecules establish their inhibition action via the adsorption of the inhibitor onto the metal surface. The adsorption processes of inhibitors are influenced by the chemical structure of organic compounds, the nature and surface change of metal, the distribution of charge in molecule and the type of aggressive media [76]. The adsorption isotherm can provide the basic information on the interaction between the inhibitor and the metal surface, which depends on the degree of surface coverage, Θ [77]. The values of surface coverage for different concentrations of inhibitor in 0.5 M solutions of pH 2 and 4 were evaluated from polarization curves according equation

The values of the degree of surface coverage are listed in Table 5. It can be seen that the values of Θ increased with an increase in the concentration of 4MBPBF_{4}. It is also worth to notice that the degree of surface coverage is higher in case of solutions of pH 4 (Table 5). Using these values of Θ, different adsorption isotherms can be used to deal with the experimental data. The Langmuir adsorption isotherm [78, 79] was applied to investigate the adsorption of 4MBPBF_{4} on copper surface given by the following equation:
where is the adsorption equilibrium constant and is the concentration of inhibitor.

Figure 8 represents the adsorption plots of 1-Butyl-4-methylpyridinium tetrafluoroborate on copper. It should be explained that other adsorption ishotherms (Frumkin and Temkin) were checked. The linear correlation coefficient was used to choose the isotherm that best fits the experimental data. It should be noted that the data fits the straight line with a slope nearly equal unity with linear correlation coefficient higher than 0.999 (Table 6) indicating that these inhibitors adsorb according to the Langmuir adsorption isotherm. The nature of corrosion inhibition has been deduced in terms of the adsorption characteristics of the inhibitor. The metal surface in aqueous solution is always covered with adsorbed water dipoles. The adsorption of inhibitor molecules from aqueous solution is a quasi-substitution process between the organic compounds in the aqueous phase and water molecules at the electrode surface [80]. The Langmuir isotherm is based on the assumption that each site of metal surface holds one adsorbed species:
In this situation, the adsorption of of one molecule of 4MBPBF_{4} is accompanied by desorption one molecule of H_{2}O from the surface of copper. This kind of isotherm involves the assumption of no interaction between the adsorbed species on the metal surface.

A graph against leads to values of , as the equilibrium constant of the adsorption process (Figure 8). The free energies of adsorption, were calculated from the adsorption equilibrium constant using the equation [81]: where value 55.5 is the molar concentration of water in the solution.

The adsorption equilibrium constant and the standard free energy of adsorption of 4BMPBF_{4} for solutions of pH 2 and 4 on copper are presented in Table 6. The values of are relatively low, meaning that interactions between 1-Butyl-4-methylpyridinium tetrafluoroborate and the metal surface are weaker. The negative values of mean that the adsorption of 4MBPBF_{4} on copper surface is a spontaneous process, and indicates the strong interaction between the inhibitor molecules and the copper surface [82].

Generally, values of around –40 kJ mol^{−1} or lower are consistent with the electrostatic interaction between the charged molecules and the charged metal surface (physisorption) [83–85]. For investigated inhibitor the values of equal −23.6 and −24.7 kJ mol^{−1} for solutions of pH 2 and 4, respectively (Table 6). The results indicate the 4MBPBF_{4} to be physically adsorbed on the copper surface. The adsorption of the inhibitor at the metal surface is the first step in the action mechanism of inhibitors in aggressive acid media. The adsorption of 1-Butyl-4-methylpyridinium tetrafluoroborate on the copper surface makes a barrier for mass and charge transfers. This situation leads to the protection of the copper surface against the attack of aggressive solution.

##### 3.6. Thermodynamic Adsorption Parameters

Thermodynamically, the free energy of adsorption, , is related to the standard enthalpy, and entropy, of the adsorption process as follows [86, 87]:
Moreover, the standard enthalpy of adsorption could be calculated according to the Van’t Hoff equation
The adsorption equilibrium constant is related to the degree of surface coverage by:
It should be noted that the decreases with increasing temperature, (Table 7). This confirms earlier made admission that the molecules of 4MBPBF_{4} are physically adsorbed on surface of copper. However, desorption process of inhibitor enhances with raising of the temperature of the solution. The free energies of adsorption of 1-Butyl-4-methylpyridinium tetrafluoroborate were calculated at different temperatures (11) and are given in Table 7. The values of are around −20 kJ mol^{−1} indicating that the adsorption mechanism of 4MBPBF_{4} in 0.5 M solution of pH 2 or 4 is physisorption at the studied temperatures.

A plot ln versus gives of straight lines, as shown in Figure 9. The slope of the straight line is. The values of the standard enthalpy are given also in Table 7. The values are negative, for that reason adsorption of 1-Butyl-4-methylpyridinium tetrafluoroborate molecules onto the Cu surface is an exothermic process. Moreover, the values of are less than −40 kJ mol^{−1} [88], therefore, once again implying that in investigated solutions, physical adsorption is taking place.

The standard entropy of inhibitor adsorption, can be calculated from (12). The values of , are recorded in Table 7. The positive values of mean that the increase in disordering takes place by going from reactants to the Cu/solution interface, which is the driving force for the adsorption of 1-Butyl-4-methylpyridinium tetrafluoroborate onto the copper surface [89].

#### 4. Conclusion

The following results can be drawn from this study.(1)The investigated 1-Butyl-4-methylpyridinium tetrafluoroborate (4MBPBF_{4}) exhibits inhibiting properties for the corrosion of copper in 0.5 M solutions of pH 2 and 4.(2)The inhibition efficiency increased with the increase in inhibitor concentration but decreases with increasing temperature. IE at all concentrations of 4MBPBF_{4} followed the order of pH: .(3)The of 1-Butyl-4-methylpyridinium tetrafluoroborate acts as a mixed-type inhibitor, independently from pH solutions.(4)The corrosion inhibition action of 1-Butyl-4-methylpyridinium tetrafluoroborate is mainly due to adsorption of 4MBPBF_{4} on the surface of copper.(5)The adsorption of the investigated compound obeys the Langmuir adsorption isotherm.(6)The thermodynamic functions of corrosion indicate that of 1-Butyl-4-methylpyridinium tetrafluoroborate adsorbs on the copper surface by a physisorption-based mechanism involving a spontaneous and exothermic process.

#### Acknowledgment

The authors would like to thank Professor M. Hepel from the Department of Chemistry SUNY at Potsdam, USA for the helpful discussions and a critical reading of the paper.

#### References

- G. Trabanelli, “Inhibitors. An old remedy for a new challenge,”
*Corrosion*, vol. 47, no. 6, pp. 410–419, 1991. View at Google Scholar · View at Scopus - A. Jardy, A. Legal Lasalle-Molin, M. Keddam, and H. Takenouti, “Copper dissolution in acidic sulphate media studied by QCM and rrde under ac signal,”
*Electrochimica Acta*, vol. 37, no. 12, pp. 2195–2201, 1992. View at Google Scholar · View at Scopus - G. Banerjee and S. N. Malhotra, “Contribution to adsorption of aromatic amines on mild steel surface from HCl solutions by impedance, UV, and Raman spectroscopy,”
*Corrosion*, vol. 48, no. 1, pp. 10–15, 1992. View at Google Scholar · View at Scopus - S. T. Arab and E. A. Noor, “Inhibition of acid corrosion of steel by some S-alkylisothiouronium iodides,”
*Corrosion*, vol. 49, no. 2, pp. 122–129, 1993. View at Google Scholar · View at Scopus - D. D. N. Singh and A. K. Dey, “Synergistic effects of inorganic and organic cations on inhibitive performance of propargyl alcohol on steel dissolution in boiling hydrochloric acid solution,”
*Corrosion*, vol. 49, no. 7, pp. 594–600, 1993. View at Google Scholar · View at Scopus - S. Martinez, “Inhibitory mechanism of mimosa tannin using molecular modeling and substitutional adsorption isotherms,”
*Materials Chemistry and Physics*, vol. 77, no. 1, pp. 97–102, 2003. View at Publisher · View at Google Scholar - M. Özcan, I. Dehri, and M. Erbil, “Organic sulphur-containing compounds as corrosion inhibitors for mild steel in acidic media: correlation between inhibition efficiency and chemical structure,”
*Applied Surface Science*, vol. 236, no. 1, pp. 155–164, 2004. View at Publisher · View at Google Scholar · View at Scopus - H. Ashassi-Sorkhabi, B. Shaabani, and D. Seifzadeh, “Effect of some pyrimidinic Shciff bases on the corrosion of mild steel in hydrochloric acid solution,”
*Electrochimica Acta*, vol. 50, no. 16-17, pp. 3446–3452, 2005. View at Publisher · View at Google Scholar · View at Scopus - J. Cruz, T. Pandiyan, and E. García-Ochoa, “A new inhibitor for mild carbon steel: electrochemical and DFT studies,”
*Journal of Electroanalytical Chemistry*, vol. 583, no. 1, pp. 8–16, 2005. View at Publisher · View at Google Scholar · View at Scopus - L. Larabi, O. Benali, S. M. Mekelleche, and Y. Harek, “2-Mercapto-1-methylimidazole as corrosion inhibitor for copper in hydrochloric acid,”
*Applied Surface Science*, vol. 253, no. 3, pp. 1371–1378, 2006. View at Publisher · View at Google Scholar · View at Scopus - J. Cruz, R. Martínez, J. Genesca, and E. García-Ochoa, “Experimental and theoretical study of 1-(2-ethylamino)-2-methylimidazoline as an inhibitor of carbon steel corrosion in acid media,”
*Journal of Electroanalytical Chemistry*, vol. 566, no. 1, pp. 111–121, 2004. View at Publisher · View at Google Scholar · View at Scopus - A. M. S. Abdennabi, A. I. Abdulhadi, S. T. Abu-Orabi, and H. Saricimen, “The inhibition action of 1(benzyl)1-H-4,5-dibenzoyl-1,2,3-triazole on mild steel in hydrochloric acid media,”
*Corrosion Science*, vol. 38, no. 10, pp. 1791–1800, 1996. View at Publisher · View at Google Scholar · View at Scopus - F. Bentiss, M. Traisnel, L. Gengembre, and M. Lagrenée, “New triazole derivative as inhibitor of the acid corrosion of mild steel: electrochemical studies, weight loss determination, SEM and XPS,”
*Applied Surface Science*, vol. 152, no. 3, pp. 237–249, 1999. View at Publisher · View at Google Scholar · View at Scopus - L. Wang, “Inhibition of mild steel corrosion in phosphoric acid solution by triazole derivatives,”
*Corrosion Science*, vol. 48, no. 3, pp. 608–616, 2006. View at Publisher · View at Google Scholar · View at Scopus - S. Kertit and B. Hammouti, “Corrosion inhibition of iron in 1M HCl by 1-phenyl-5-mercapto-1,2,3,4-tetrazole,”
*Applied Surface Science*, vol. 93, no. 1, pp. 59–66, 1996. View at Publisher · View at Google Scholar · View at Scopus - R. M. Hudson, T. J. Butler, and C. J. Warning, “The effect of pyrrole-halide mixtures in inhibiting the dissolution of low-carbon steel in sulphuric acid,”
*Corrosion Science*, vol. 17, no. 7, pp. 571–581, 1977. View at Google Scholar · View at Scopus - M. A. Veloz and I. G. Martínez, “Effect of some pyridine derivatives on the corrosion behavior of carbon steel in an environment like NAGE TM0177,”
*Corrosion*, vol. 62, no. 4, pp. 283–292, 2006. View at Google Scholar · View at Scopus - A. Ouchrif, M. Zegmout, B. Hammouti, S. El-Kadiri, and A. Ramdani, “1,3-Bis(3-hyroxymethyl-5-methyl-1-pyrazole) propane as corrosion inhibitor for steel in 0.5 M H
_{2}SO_{4}solution,”*Applied Surface Science*, vol. 252, no. 2, pp. 339–344, 2005. View at Publisher · View at Google Scholar · View at Scopus - A. Chetouani, B. Hammouti, T. Benhadda, and M. Daoudi, “Inhibitive action of bipyrazolic type organic compounds towards corrosion of pure iron in acidic media,”
*Applied Surface Science*, vol. 249, no. 1–4, pp. 375–385, 2005. View at Publisher · View at Google Scholar · View at Scopus - S. A. Abd El-Maksoud, “The influence of some Arylazobenzoyl acetonitrile derivatives on the behaviour of carbon steel in acidic media,”
*Applied Surface Science*, vol. 206, no. 1–4, pp. 129–136, 2003. View at Publisher · View at Google Scholar - A. Chetouani, A. Aouniti, B. Hammouti, N. Benchat, T. Benhadda, and S. Kertit, “Corrosion inhibitors for iron in hydrochloride acid solution by newly synthesised pyridazine derivatives,”
*Corrosion Science*, vol. 45, no. 8, pp. 1675–1684, 2003. View at Publisher · View at Google Scholar · View at Scopus - M. Ohsawa and W. Suëtaka, “Spectro-electrochemical studies of the corrosion inhibition of copper by mercaptobenzothiazole,”
*Corrosion Science*, vol. 19, no. 7, pp. 709–722, 1979. View at Google Scholar · View at Scopus - G. W. Walter, “A review of impedance plot methods used for corrosion performance analysis of painted metals,”
*Corrosion Science*, vol. 26, no. 9, pp. 681–703, 1986. View at Google Scholar · View at Scopus - B. Trachli, M. Keddam, H. Takenouti, and A. Srhiri, “Protective effect of electropolymerized 3-amino 1,2,4-triazole towards corrosion of copper in 0.5 M NaCl,”
*Corrosion Science*, vol. 44, no. 5, pp. 997–1008, 2002. View at Publisher · View at Google Scholar · View at Scopus - M. Hepel and M. Scendo, “Growth kinetics of multi-layer CuEtX films on copper piezoelectrodes,” in
*Thin Films: Preparation, Characterization, Applications*, M. P. Soriaga, J. Stickney, L. A. Bottomley, and Y.-G. Kim, Eds., Kluwer Academic/Plenum Publishers, New York, NY, USA, 2001. View at Google Scholar - M. Hepel and M. Scendo, “Kinetics of CuEtX film formation on copper piezoelectrodes,”
*Journal of Electroanalytical Chemistry*, vol. 538-539, pp. 121–132, 2002. View at Publisher · View at Google Scholar · View at Scopus - M. Scendo, “Potassium ethyl xanthate as corrosion inhibitor for copper in acidic chloride solutions,”
*Corrosion Science*, vol. 47, no. 7, pp. 1738–1749, 2005. View at Publisher · View at Google Scholar · View at Scopus - M. Scendo, “Corrosion inhibition of copper by potassium ethyl xanthate in acidic chloride solutions,”
*Corrosion Science*, vol. 47, no. 11, pp. 2778–2791, 2005. View at Publisher · View at Google Scholar · View at Scopus - M. Scendo, D. Poddebniak, and J. Malyszko, “Indole and 5-chloroindole as inhibitors of anodic dissolution and cathodic deposition of copper in acidic chloride solutions,”
*Journal of Applied Electrochemistry*, vol. 33, no. 3-4, pp. 287–293, 2003. View at Publisher · View at Google Scholar · View at Scopus - A. A. Aksüt and S. Bilgiç, “The effect of amino acids on the corrosion of nickel in H
_{2}SO_{4},”*Corrosion Science*, vol. 33, no. 3, pp. 379–387, 1992. View at Google Scholar - H. Baba and T. Kodama, “Corrosion inhibition and characteristics of the triazinedithiol surface film on copper under potentiostatic anodization,”
*Corrosion Science*, vol. 41, no. 10, pp. 1987–2000, 1999. View at Publisher · View at Google Scholar · View at Scopus - G. Moretti and F. Guidi, “Tryptophan as copper corrosion inhibitor in 0.5 M aerated sulfuric acid,”
*Corrosion Science*, vol. 44, no. 9, pp. 1995–2011, 2002. View at Publisher · View at Google Scholar · View at Scopus - J. B. Matos, L. P. Pereira, S. M. L. Agostinho, O. E. Barcia, G. G. O. Cordeiro, and E. D'Elia, “Effect of cysteine on the anodic dissolution of copper in sulfuric acid medium,”
*Journal of Electroanalytical Chemistry*, vol. 570, no. 1, pp. 91–94, 2004. View at Publisher · View at Google Scholar · View at Scopus - M. Scendo, “The effect of purine on the corrosion of copper in chloride solutions,”
*Corrosion Science*, vol. 49, no. 2, pp. 373–390, 2007. View at Publisher · View at Google Scholar · View at Scopus - M. Scendo, “The influence of adenine on corrosion of copper in chloride solutions,”
*Corrosion Science*, vol. 50, no. 7, pp. 2070–2077, 2008. View at Publisher · View at Google Scholar · View at Scopus - M. Scendo, “Inhibitive action of the purine and adenine for copper corrosion in sulphate solutions,”
*Corrosion Science*, vol. 49, no. 7, pp. 2985–3000, 2007. View at Publisher · View at Google Scholar · View at Scopus - M. Scendo, “Inhibition of copper corrosion in sodium nitrate solutions with nontoxic inhibitors,”
*Corrosion Science*, vol. 50, no. 6, pp. 1584–1592, 2008. View at Publisher · View at Google Scholar · View at Scopus - S. Muralidharan and S. Venkatakrishna Iyer, “The influence of N-heterocyclics on corrosion inhibition and hydrogen permeation through mild steel in acidic solutions,”
*Anti-Corrosion Methods and Materials*, vol. 44, no. 2, pp. 100–106, 1997. View at Google Scholar - R. Gašparac, C. R. Martin, and E. Stupnišek-Lisac, “In situ studies of imidazole and its derivatives as copper corrosion inhibitors I. Activation energies and thermodynamics of adsorption,”
*Journal of the Electrochemical Society*, vol. 147, no. 2, pp. 548–551, 2000. View at Publisher · View at Google Scholar · View at Scopus - D. Q. Zhang, L. X. Gao, and G. D. Zhou, “Inhibition of copper corrosion in aerated hydrochloric acid solution by heterocyclic compounds containing a mercapto group,”
*Corrosion Science*, vol. 46, no. 12, pp. 3031–3040, 2004. View at Publisher · View at Google Scholar · View at Scopus - M. A. Quraishi, M. Z. A. Rafiquee, S. Khan, and N. Saxena, “Corrosion inhibition of aluminium in acid solutions by some imidazoline derivatives,”
*Journal of Applied Electrochemistry*, vol. 37, no. 10, pp. 1153–1162, 2007. View at Publisher · View at Google Scholar · View at Scopus - S. Caporali, A. Fossati, A. Lavacchi, I. Perissi, A. Tolstogouzov, and U. Bardi, “Aluminium electroplated from ionic liquids as protective coating against steel corrosion,”
*Corrosion Science*, vol. 50, no. 2, pp. 534–539, 2008. View at Publisher · View at Google Scholar · View at Scopus - G. Yue, X. Lu, Y. Zhu, X. Zhang, and S. Zhang, “Surface morphology, crystal structure and orientation of aluminium coatings electrodeposited on mild steel in ionic liquid,”
*Chemical Engineering Journal*, vol. 147, no. 1, pp. 79–86, 2009. View at Publisher · View at Google Scholar - A. Inglese, P. D'Angelo, R. De Lisi, and S. Milioto, “Surface tension, heat capacity, and volume of amphiphilic compounds in formamide solutions,”
*Journal of Solution Chemistry*, vol. 27, no. 5, pp. 403–424, 1998. View at Google Scholar · View at Scopus - P. Zhao, C. Zhong, L. Hunag, L. Niu, and F. Zhang, “Corrosion inhibition of dibenzo [1,4,8,11] tetraaza [14] annulene nickel on steel in 1 M HCl,”
*Corrosion Science*, vol. 50, no. 8, pp. 2166–2171, 2008. View at Publisher · View at Google Scholar · View at Scopus - N. Kimizuka and T. Nakashima, “Spontaneous self-assembly of glycolipid bilayer membranes in sugar-philic ionic liquids and formation of ionogels,”
*Langmuir*, vol. 17, no. 22, pp. 6759–6761, 2001. View at Publisher · View at Google Scholar · View at Scopus - L. C. Branco, J. N. Rosa, J. J. Moura Ramos, and C. A. M. Afonso, “Preparation and characterization of new room temperature ionic liquids,”
*Chemistry*, vol. 8, no. 16, pp. 3671–3677, 2002. View at Google Scholar · View at Scopus - J. Pernak, K. Sobaszkiewicz, and J. Foksowicz-Flaczyk, “Ionic liquids with symmetrical dialkoxymethyl-substituted imidazolium cations,”
*Chemistry*, vol. 10, no. 14, pp. 3479–3485, 2004. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - Z. B. Zhou, H. Matsumoto, and K. Tatsumi, “Low-melting, low-viscous, hydrophobic ionic liquids: 1-Alkyl(alkyl ether)-3-methylimidazolium perfluoroalkyltrifluoroborate,”
*Chemistry*, vol. 10, no. 24, pp. 6581–6591, 2004. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - Q. Liu, M. H. A. Janssen, F. Van Rantwijk, and R. A. Sheldon, “Room-temperature ionic liquids that dissolve carbohydrates in high concentrations,”
*Green Chemistry*, vol. 7, no. 1, pp. 39–42, 2005. View at Publisher · View at Google Scholar · View at Scopus - W. A. Henderson, V. G. Young, D. M. Fox, H. C. De Long, and P. C. Trulove, “Alkyl vs. alkoxy chains on ionic liquid cations,”
*Chemical Communications*, no. 35, pp. 3708–3710, 2006. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - Z. Fei, W. H. Ang, D. Zhao et al., “Revisiting ether-derivatized imidazolium-based ionic liquids,”
*Journal of Physical Chemistry B*, vol. 111, no. 34, pp. 10095–10108, 2007. View at Publisher · View at Google Scholar · View at Scopus - J. Malyszko and M. Scendo, “Redox equilibria in the Cu
^{2+}-Cu^{+}-Cu system in water-dimethylsulphoxide (DMSO) mixtures,”*Monatshefte für Chemie Chemical Monthly*, vol. 118, no. 4, pp. 435–443, 1987. View at Publisher · View at Google Scholar · View at Scopus - J. Matyszko and M. Scendo, “The stepwise reduction of Cu(II) at a platinum electrode in water +
*N,N*-dimethylformamide mixtures,”*Journal of Electroanalytical Chemistry*, vol. 269, no. 1, pp. 113–128, 1989. View at Google Scholar · View at Scopus - J. Małyszko and M. Scendo, “Electrode kinetics of the Cu(II)/Cu(I) system at platinum in water + dimethylsulphoxide (DMSO) mixtures,”
*Journal of Electroanalytical Chemistry*, vol. 250, no. 1, pp. 61–72, 1988. View at Google Scholar · View at Scopus - M. Scendo and J. Malyszko, “Influence of benzotriazole and tolyltriazole on the copper electrodeposition on polycrystalline platinum from acidic chloride solutions,”
*Journal of the Electrochemical Society*, vol. 147, no. 5, pp. 1758–1762, 2000. View at Publisher · View at Google Scholar · View at Scopus - S. S. Abdel-Rehim, A. M. Magdy, and K. F. Khaled, “The inhibition of 4-(${2}^{\prime}$-amino-${5}^{\prime}$-methylphenylazo) antipyrine on corrosion of mild steel in HCl solution,”
*Materials Chemistry and Physics*, vol. 70, no. 3, pp. 268–273, 2001. View at Google Scholar - M. Elachouri, M. S. Hajji, M. Salem et al., “Some nonionic surfactants as inhibitors of the corrosion of iron in acid chloride solutions,”
*Corrosion*, vol. 52, no. 2, pp. 103–108, 1996. View at Google Scholar · View at Scopus - B. R. Babu and R. Holze, “Corrosion and hydrogen permeation inhibition for mild steel in HCl by isomers of organic compounds,”
*British Corrosion Journal*, vol. 35, no. 3, pp. 204–209, 2000. View at Google Scholar · View at Scopus - V. Shinde, S. R. Sainkar, and P. P. Patil, “Corrosion protective poly(o-toluidine) coatings on copper,”
*Corrosion Science*, vol. 47, no. 6, pp. 1352–1369, 2005. View at Publisher · View at Google Scholar · View at Scopus - D. W. Suggs and A. J. Bard, “Scanning tunneling microscopic study with atomic resolution of the dissolution of Cu(100) electrodes in aqueous chloride media,”
*Journal of Physical Chemistry*, vol. 99, no. 20, pp. 8349–8355, 1995. View at Google Scholar · View at Scopus - G. M. Brisard, E. Zenati, H. A. Gasteiger, N. M. Marković, and P. N. Ross, “Underpotential deposition of lead on Cu(100) in the presence of chloride:
*ex-situ*low-energy electron diffraction, auger electron spectroscopy, and electrochemical studies,”*Langmuir*, vol. 13, no. 8, pp. 2390–2397, 1997. View at Google Scholar · View at Scopus - G. Brisard, N. Bertrand, P. N. Ross, and N. M. Marković, “Oxygen reduction and hydrogen evolution-oxidation reactions on Cu(hkl) surfaces,”
*Journal of Electroanalytical Chemistry*, vol. 480, no. 1-2, pp. 219–224, 2000. View at Publisher · View at Google Scholar · View at Scopus - H. Ma, S. Chen, B. Yin, S. Zhao, and X. Liu, “Impedance spectrospic study of corrosion inhibition of copper by surfactants in the acidic solutions,”
*Corrosion Science*, vol. 45, no. 5, pp. 867–882, 2003. View at Publisher · View at Google Scholar · View at Scopus - D. Hang, L. Gao, G. Zhou, and K. Y. Lee, “Undecyl substitution in imidazole and its action on corrosion inhibition of copper in aerated acidic chloride media,”
*Journal of Applied Electrochemistry*, vol. 38, pp. 71–76, 2008. View at Google Scholar - E. Yeager, “Electrocatalysts for O
_{2}reduction,”*Electrochimica Acta*, vol. 29, no. 11, pp. 1527–1537, 1984. View at Google Scholar · View at Scopus - D. Pletcher and S. Sotiropoulos, “A study of cathodic oxygen reduction at platinum using microelectrodes,”
*Journal of Electroanalytical Chemistry*, vol. 356, no. 1-2, pp. 109–119, 1993. View at Google Scholar · View at Scopus - A. H. Moreira, A. V. Benedetti, P. L. Cabot, and P. T. A. Sumodjo, “Electrochemical behaviour of copper electrode in concentrated sulfuric acid solutions,”
*Electrochimica Acta*, vol. 38, no. 7, pp. 981–987, 1993. View at Google Scholar · View at Scopus - H. P. Lee and K. Nobe, “Kinetics and mechanisms of Cu electrodissolution in chloride media,”
*Journal of the Electrochemical Society*, vol. 133, no. 10, pp. 2035–2043, 1986. View at Google Scholar · View at Scopus - F. K. Crundwell, “The anodic dissolution of copper in hydrochloric acid solutions,”
*Electrochimica Acta*, vol. 37, no. 15, pp. 2707–2714, 1992. View at Google Scholar · View at Scopus - E. A. Noor and A. H. Al-Moubaraki, “Thermodynamic study of metal corrosion and inhibitor adsorption processes in mild steel/1-methyl-4[${2}^{\prime}$(-X)-styryl pyridinium iodides/hydrochloric acid systems,”
*Materials Chemistry and Physics*, vol. 110, no. 1, pp. 145–154, 2008. View at Publisher · View at Google Scholar · View at Scopus - V. R. Saliyan and A. V. Adhikari, “Quinolin-5-ylmethylene-3-{[8-(trifluoromethyl)quinolin-4-yl]thio}propanohydrazide as an effective inhibitor of mild steel corrosion in HCl solution,”
*Corrosion Science*, vol. 50, no. 1, pp. 55–61, 2008. View at Publisher · View at Google Scholar · View at Scopus - S. S. Abd El Rehim, H. H. Hassan, and M. A. Amin, “Corrosion inhibition of aluminum by 1,1(lauryl amido)propyl ammonium chloride in HCl solution,”
*Materials Chemistry and Physics*, vol. 70, no. 1, pp. 64–72, 2001. View at Publisher · View at Google Scholar · View at Scopus - S. T. Arb and K. M. Emran, “Thermodynamic study on corrosion inhibition of Fe78B13Si9 metallic glass alloy in Na2SO4 solution at different temperatures,”
*International Journal of Applied Chemistry*, vol. 3, pp. 69–77, 2007. View at Google Scholar - G. K. Gomma and M. H. Wahdan, “Schiff bases as corrosion inhibitors for aluminium in hydrochloric acid solution,”
*Materials Chemistry & Physics*, vol. 39, no. 3, pp. 209–213, 1995. View at Google Scholar · View at Scopus - A. K. Maayta and N. A. F. Al-Rawashdeh, “Inhibition of acidic corrosion of pure aluminum by some organic compounds,”
*Corrosion Science*, vol. 46, no. 5, pp. 1129–1140, 2004. View at Publisher · View at Google Scholar · View at Scopus - M. Lagrenée, B. Mernari, M. Bouanis, M. Traisnel, and F. Bentiss, “Study of the mechanism and inhibiting efficiency of 3,5-bis(4-methylthiophenyl)-4H-1,2,4-triazole on mild steel corrosion in acidic media,”
*Corrosion Science*, vol. 44, no. 3, pp. 573–588, 2002. View at Publisher · View at Google Scholar - G. N. Mu, T. P. Zhao, M. Liu, and T. Gu, “Effect of metallic cations on corrosion inhibition of an anionic surfactant for mild steel,”
*Corrosion*, vol. 52, no. 11, pp. 853–856, 1996. View at Google Scholar · View at Scopus - F. Bentiss, M. Lagrenée, B. Elmehdi, B. Mernari, M. Traisnel, and H. Vezin, “Electrochemical and quantum chemical studies of 3,5-Di (n-Tolyl)-4-amino-1,2,4-triazole adsorption on mild steel in acidic media,”
*Corrosion*, vol. 58, no. 5, pp. 399–407, 2002. View at Google Scholar · View at Scopus - M. Şahin, S. Bilgiç, and H. Yilmaz, “The inhibition effects of some cyclic nitrogen compounds on the corrosion of the steel in NaCl mediums,”
*Applied Surface Science*, vol. 195, no. 1–4, pp. 1–7, 2002. View at Publisher · View at Google Scholar · View at Scopus - X. Li, L. Tang, H. Liu, G. Mu, and G. Liu, “Influence of halide ions on inhibitive performance of cetyl trimethyl ammonium bromide in various concentrations of phosphoric acid for cold rolled steel,”
*Materials Letters*, vol. 62, no. 15, pp. 2321–2324, 2008. View at Publisher · View at Google Scholar · View at Scopus - B. V. Savithri and S. M. Mayanna, “Tetrabutyl ammonium iodide, cetyl pyridinium bromide and cetyl trimethyl ammonium bromide as corrosion inhibitors for mild steel in sulphuric acid,”
*Indian Journal of Chemical Technology*, vol. 3, no. 5, pp. 256–258, 1996. View at Google Scholar · View at Scopus - F. Bensajjay, S. Alehyen, M. El Achouri, and S. Kertit, “Corrosion inhibition of steel by 1-phenyl 5-mercapto 1,2,3,4-tetrazole in acidic environments (0.5 M H
_{2}SO_{4}and 1/3 M HPO),”*Anti-Corrosion Methods and Materials*, vol. 50, no. 6, pp. 402–409, 2003. View at Publisher · View at Google Scholar · View at Scopus - F. Bentiss, M. Lebrini, and M. Lagrenée, “Thermodynamic characterization of metal dissolution and inhibitor adsorption processes in mild steel/2,5-bis(n-thienyl)-1,3,4-thiadiazoles/ hydrochloric acid system,”
*Corrosion Science*, vol. 47, no. 12, pp. 2915–2931, 2005. View at Publisher · View at Google Scholar · View at Scopus - W. H. Li, Q. He, S. T. Zhang, C. L. Pei, and B. R. Hou, “Some new triazole derivatives as inhibitors for mild steel corrosion in acidic medium,”
*Journal of Applied Electrochemistry*, vol. 38, no. 3, pp. 289–295, 2008. View at Publisher · View at Google Scholar · View at Scopus - X. Li and G. Mu, “Tween-40 as corrosion inhibitor for cold rolled steel in sulphuric acid: weight loss study, electrochemical characterization, and AFM,”
*Applied Surface Science*, vol. 252, no. 5, pp. 1254–1265, 2005. View at Publisher · View at Google Scholar · View at Scopus - M. Bouklah, B. Hammouti, M. Lagrenée, and F. Bentiss, “Thermodynamic properties of 2,5-bis(4-methoxyphenyl)-1,3,4-oxadiazole as a corrosion inhibitor for mild steel in normal sulfuric acid medium,”
*Corrosion Science*, vol. 48, no. 9, pp. 2831–2842, 2006. View at Publisher · View at Google Scholar · View at Scopus - M. Benabdellah, R. Touzani, A. Dafali, B. Hammouti, and S. El Kadiri, “Ruthenium-ligand complex, an efficient inhibitor of steel corrosion in H
_{3}PO_{4}media,”*Materials Letters*, vol. 61, no. 4-5, pp. 1197–1204, 2007. View at Publisher · View at Google Scholar · View at Scopus - X. Li, S. Deng, G. Mu, H. Fu, and F. Yang, “Inhibition effect of nonionic surfactant on the corrosion of cold rolled steel in hydrochloric acid,”
*Corrosion Science*, vol. 50, no. 2, pp. 420–430, 2008. View at Publisher · View at Google Scholar